#------------------------------------------------------------------------------
#$Date: 2016-02-16 03:10:39 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/00/17/7001789.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7001789
loop_
_publ_author_name
'Shi, Shu-Yun'
'Wang, Yan'
'Cui, Xiao-Bing'
'Wang, Guo-Wu'
'Yang, Guang-Di'
'Xu, Ji-Qing'
_publ_section_title
;
 Synthesis and characterization of a novel POM compound containing two
 different layers stacked alternately
;
_journal_issue                   31
_journal_name_full               'Dalton Transactions'
_journal_page_first              6099
_journal_paper_doi               10.1039/b906066a
_journal_year                    2009
_chemical_formula_sum            'C5 H41 Mo24 N5 O88.5 Sb4 Si2'
_chemical_formula_weight         4433.17
_chemical_name_systematic
;
?
;
_space_group_IT_number           5
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 104.37(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   20.544(4)
_cell_length_b                   20.438(4)
_cell_length_c                   20.551(4)
_cell_measurement_temperature    293(2)
_cell_volume                     8359(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0362
_diffrn_reflns_av_sigmaI/netI    0.0553
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            33768
_diffrn_reflns_theta_full        26.05
_diffrn_reflns_theta_max         26.05
_diffrn_reflns_theta_min         2.24
_exptl_absorpt_coefficient_mu    4.889
_exptl_absorpt_correction_T_max  0.2728
_exptl_absorpt_correction_T_min  0.1360
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    3.523
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             8216
_exptl_crystal_size_max          0.68
_exptl_crystal_size_mid          0.36
_exptl_crystal_size_min          0.36
_refine_diff_density_max         2.326
_refine_diff_density_min         -4.429
_refine_diff_density_rms         0.330
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.52(5)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.092
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1090
_refine_ls_number_reflns         16355
_refine_ls_number_restraints     196
_refine_ls_restrained_S_all      1.090
_refine_ls_R_factor_all          0.0672
_refine_ls_R_factor_gt           0.0539
_refine_ls_shift/su_max          0.016
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1675
_refine_ls_wR_factor_ref         0.1775
_reflns_number_gt                12658
_reflns_number_total             16355
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b906066a.txt
_cod_data_source_block           k
_cod_original_sg_symbol_H-M      C2
_cod_original_formula_sum        'C5 H41 Mo24 N5 O88.50 Sb4 Si2'
_cod_database_code               7001789
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo -0.54208(8) 0.60010(9) -0.13141(8) 0.0152(4) Uani 1 1 d . . .
Mo2 Mo -0.65869(7) 0.48711(12) -0.12563(7) 0.0201(4) Uani 1 1 d . . .
Mo3 Mo -0.40938(7) 0.47906(12) -0.13050(7) 0.0188(4) Uani 1 1 d . . .
Mo4 Mo -0.62908(8) 0.60030(9) -0.00363(8) 0.0157(4) Uani 1 1 d . . .
Mo5 Mo -0.52858(8) 0.36583(9) -0.13203(8) 0.0155(4) Uani 1 1 d . . .
Mo6 Mo -0.37458(8) 0.36617(9) -0.00965(8) 0.0148(4) Uani 1 1 d . . .
Mo7 Mo -0.91585(7) 0.47656(11) -0.13174(6) 0.0155(4) Uani 1 1 d . . .
Mo8 Mo -1.03654(9) 0.60819(10) -0.12763(8) 0.0186(4) Uani 1 1 d . . .
Mo9 Mo -0.88539(9) 0.35487(9) -0.00743(8) 0.0153(4) Uani 1 1 d . . .
Mo10 Mo -1.02861(9) 0.35768(11) -0.12854(8) 0.0212(4) Uani 1 1 d . . .
Mo11 Mo -1.15047(7) 0.48963(10) -0.13186(6) 0.0145(4) Uani 1 1 d . . .
Mo12 Mo -1.11861(8) 0.61180(9) -0.00548(8) 0.0142(4) Uani 1 1 d . . .
Mo13 Mo -0.90431(8) 0.20943(11) -0.62808(8) 0.0256(4) Uani 1 1 d . . .
Mo14 Mo -0.72219(8) 0.33723(11) -0.36912(8) 0.0228(4) Uani 1 1 d . . .
Mo15 Mo -0.77800(8) 0.33683(11) -0.62914(8) 0.0234(4) Uani 1 1 d . . .
Mo16 Mo -0.86998(9) 0.33824(10) -0.48975(8) 0.0240(4) Uani 1 1 d . . .
Mo17 Mo -0.62438(8) 0.09364(10) -0.49314(8) 0.0243(4) Uani 1 1 d . . .
Mo18 Mo -0.87318(9) 0.09204(11) -0.50513(8) 0.0267(5) Uani 1 1 d . . .
Mo19 Mo -0.63020(9) 0.33936(10) -0.50838(8) 0.0231(4) Uani 1 1 d . . .
Mo20 Mo -0.59430(8) 0.21065(11) -0.36998(8) 0.0239(4) Uani 1 1 d . . .
Mo21 Mo -0.66201(9) 0.22229(11) -0.63018(8) 0.0219(4) Uani 1 1 d . . .
Mo22 Mo -0.83703(9) 0.22131(11) -0.36848(8) 0.0219(4) Uani 1 1 d . . .
Mo23 Mo -0.78947(9) 0.09541(10) -0.62853(8) 0.0241(5) Uani 1 1 d . . .
Mo24 Mo -0.70807(9) 0.09569(10) -0.36966(8) 0.0234(4) Uani 1 1 d . . .
Sb1 Sb -0.5000 0.26797(9) 0.0000 0.0150(4) Uani 1 2 d S . .
Sb2 Sb -0.78587(4) 0.48262(8) -0.00047(4) 0.0138(2) Uani 1 1 d . . .
Sb3 Sb -0.53465(13) 0.21693(16) -0.50008(13) 0.0315(6) Uani 0.50 1 d P . .
Sb4 Sb -0.96336(13) 0.21570(16) -0.49839(14) 0.0332(6) Uani 0.50 1 d P . .
Sb5 Sb -0.75098(12) 0.43141(16) -0.49943(12) 0.0303(7) Uani 0.50 1 d P . .
Sb6 Sb -0.75182(12) 0.50179(16) -0.50123(12) 0.0330(7) Uani 0.50 1 d P . .
Sb7 Sb -0.5000 0.69765(9) 0.0000 0.0144(4) Uani 1 2 d S . .
Si1 Si -0.5000 0.4810(5) 0.0000 0.0155(15) Uani 1 2 d S . .
Si2 Si -1.0000 0.4816(5) 0.0000 0.0167(15) Uani 1 2 d S . .
Si3 Si -0.74890(19) 0.2145(4) -0.49906(18) 0.0109(13) Uani 1 1 d . . .
O1 O -0.4867(7) 0.5403(7) -0.1539(6) 0.030(4) Uani 1 1 d . . .
O2 O -0.4669(6) 0.4393(7) -0.0499(6) 0.020(3) Uani 1 1 d U . .
O3 O -0.3687(6) 0.4896(10) -0.1886(6) 0.039(4) Uani 1 1 d . . .
O4 O -0.7268(7) 0.4669(9) -0.1808(6) 0.041(4) Uani 1 1 d . . .
O5 O -0.5386(7) 0.6603(9) -0.1866(7) 0.037(4) Uani 1 1 d U . .
O6 O -0.3174(7) 0.3046(7) 0.0052(6) 0.028(4) Uani 1 1 d . . .
O7 O -0.6805(7) 0.6566(8) 0.0129(6) 0.028(3) Uani 1 1 d . . .
O8 O -0.6899(6) 0.5605(8) -0.0782(6) 0.028(3) Uani 1 1 d . . .
O9 O -0.4631(6) 0.6342(6) -0.0560(6) 0.014(3) Uani 1 1 d U . .
O10 O -0.3700(5) 0.5393(7) -0.0634(5) 0.020(3) Uani 1 1 d U . .
O11 O -0.6207(7) 0.5556(9) -0.1710(6) 0.039(4) Uani 1 1 d . . .
O12 O -0.3505(6) 0.4093(8) -0.0838(5) 0.027(3) Uani 1 1 d . . .
O13 O -0.6615(6) 0.4289(7) -0.0516(5) 0.020(3) Uani 1 1 d . . .
O14 O -0.5589(7) 0.3014(8) -0.1875(8) 0.034(4) Uani 1 1 d . . .
O15 O -0.5851(6) 0.6491(7) -0.0670(6) 0.027(3) Uani 1 1 d . . .
O16 O -0.5928(6) 0.4278(7) -0.1482(5) 0.020(3) Uani 1 1 d U . .
O17 O -0.4535(6) 0.3088(7) -0.0732(6) 0.026(3) Uani 1 1 d . . .
O18 O -0.5563(5) 0.5291(6) -0.0449(5) 0.011(2) Uani 1 1 d U . .
O19 O -0.5654(6) 0.3318(7) -0.0532(6) 0.016(3) Uani 1 1 d . . .
O20 O -0.4709(6) 0.4068(8) -0.1743(5) 0.023(3) Uani 1 1 d . . .
O21 O -1.0335(7) 0.6638(9) -0.1838(7) 0.039(4) Uani 1 1 d . . .
O22 O -1.1750(6) 0.6647(8) 0.0126(6) 0.030(3) Uani 1 1 d U . .
O23 O -1.2242(5) 0.4699(8) -0.1838(5) 0.027(3) Uani 1 1 d U . .
O24 O -1.0579(7) 0.2973(7) -0.1870(7) 0.026(3) Uani 1 1 d . . .
O25 O -0.8721(5) 0.4889(9) -0.1889(5) 0.032(3) Uani 1 1 d U . .
O26 O -0.9579(6) 0.6319(6) -0.0592(5) 0.015(3) Uani 1 1 d U . .
O27 O -1.0555(5) 0.5305(6) -0.0454(5) 0.015(3) Uani 1 1 d U . .
O28 O -0.8213(6) 0.2997(7) 0.0093(5) 0.018(3) Uani 1 1 d U . .
O29 O -0.8114(6) 0.5492(8) 0.0700(7) 0.033(4) Uani 1 1 d . . .
O30 O -0.8653(6) 0.5354(7) -0.0579(6) 0.020(3) Uani 1 1 d . . .
O31 O -0.9459(7) 0.3116(6) -0.0800(6) 0.025(3) Uani 1 1 d . . .
O32 O -0.9658(5) 0.4394(7) -0.0479(6) 0.017(3) Uani 1 1 d . . .
O33 O -1.1155(7) 0.5580(7) -0.1732(6) 0.036(4) Uani 1 1 d . . .
O34 O -1.0956(6) 0.6510(7) -0.0793(6) 0.026(3) Uani 1 1 d . . .
O35 O -0.8462(6) 0.4174(8) -0.0713(6) 0.024(3) Uani 1 1 d U . .
O36 O -0.8375(6) 0.4338(7) 0.0512(5) 0.018(3) Uani 1 1 d U . .
O37 O -0.9832(6) 0.5381(7) -0.1493(6) 0.023(3) Uani 1 1 d U . .
O38 O -0.9708(7) 0.4088(8) -0.1723(6) 0.028(3) Uani 1 1 d U . .
O39 O -1.0926(6) 0.4281(7) -0.1486(5) 0.024(3) Uani 1 1 d U . .
O40 O -0.9278(5) 0.3374(6) 0.0573(5) 0.012(3) Uani 1 1 d U . .
O41 O -0.6892(7) 0.3884(7) -0.3086(6) 0.031(3) Uani 1 1 d U . .
O42 O -0.8978(7) 0.2899(8) -0.4242(6) 0.034(4) Uani 1 1 d . . .
O43 O -0.6980(6) 0.3843(8) -0.5733(6) 0.029(4) Uani 1 1 d . . .
O44 O -0.7929(8) 0.5702(7) -0.4477(7) 0.038(4) Uani 1 1 d . . .
O45 O -0.9290(8) 0.3934(8) -0.5061(7) 0.049(5) Uani 1 1 d . . .
O46 O -0.9245(7) 0.0326(7) -0.4887(7) 0.036(4) Uani 1 1 d U . .
O47 O -0.8763(6) 0.2002(7) -0.3062(5) 0.028(3) Uani 1 1 d . . .
O48 O -0.7916(7) 0.0364(8) -0.6875(7) 0.038(4) Uani 1 1 d . . .
O49 O -0.6201(6) 0.2017(7) -0.6904(6) 0.034(4) Uani 1 1 d . . .
O50 O -0.5741(7) 0.0357(7) -0.5104(7) 0.036(4) Uani 1 1 d . . .
O51 O -0.5209(6) 0.2245(9) -0.3129(7) 0.036(4) Uani 1 1 d . . .
O52 O -0.9800(7) 0.2237(9) -0.6842(6) 0.035(4) Uani 1 1 d . . .
O53 O -0.6133(7) 0.1612(8) -0.5513(6) 0.032(4) Uani 1 1 d U . .
O54 O -0.8032(6) 0.3836(8) -0.4241(6) 0.031(4) Uani 1 1 d U . .
O55 O -0.7058(7) 0.0359(7) -0.3120(6) 0.029(3) Uani 1 1 d . . .
O56 O -0.8120(7) 0.3897(7) -0.6866(6) 0.031(3) Uani 1 1 d . . .
O57 O -0.5668(7) 0.3962(8) -0.4906(7) 0.037(4) Uani 1 1 d . . .
O58 O -0.8106(7) 0.1716(8) -0.5485(6) 0.032(4) Uani 1 1 d . . .
O59 O -0.7143(8) 0.5718(9) -0.5573(8) 0.043(5) Uani 1 1 d . . .
O60 O -0.6022(7) 0.2902(8) -0.5735(6) 0.028(3) Uani 1 1 d U . .
O61 O -0.6591(7) 0.5428(8) -0.4287(6) 0.033(3) Uani 1 1 d U . .
O62 O -0.6892(6) 0.1708(8) -0.4498(6) 0.023(3) Uani 1 1 d U . .
O63 O -0.7829(6) 0.2644(7) -0.4517(6) 0.021(3) Uani 1 1 d U . .
O64 O -0.9117(6) 0.2744(7) -0.5545(6) 0.026(3) Uani 1 1 d U . .
O65 O -0.5627(6) 0.1436(7) -0.4287(5) 0.021(3) Uiso 1 1 d . . .
O66 O -0.8714(5) 0.1376(7) -0.6702(5) 0.020(3) Uani 1 1 d . . .
O67 O -0.7655(7) 0.1608(8) -0.3494(5) 0.030(4) Uani 1 1 d . . .
O68 O -0.5873(6) 0.2733(7) -0.4404(6) 0.025(3) Uani 1 1 d . . .
O69 O -0.6260(5) 0.1386(6) -0.3281(5) 0.016(3) Uiso 1 1 d . . .
O70 O -0.7160(6) 0.2650(7) -0.5463(5) 0.018(3) Uani 1 1 d U . .
O71 O -0.7191(6) 0.2926(8) -0.6740(6) 0.027(3) Uani 1 1 d U . .
O72 O -0.7807(7) 0.2896(7) -0.3245(6) 0.027(3) Uani 1 1 d . . .
O73 O -0.8427(6) 0.5434(7) -0.5727(6) 0.025(3) Uani 1 1 d U . .
O74 O -0.8849(7) 0.1623(9) -0.4455(6) 0.032(4) Uani 1 1 d . . .
O75 O -0.8466(6) 0.2708(8) -0.6506(6) 0.029(3) Uani 1 1 d . . .
O76 O -0.7311(6) 0.1618(7) -0.6499(5) 0.020(3) Uani 1 1 d . . .
O77 O -0.6532(6) 0.2715(8) -0.3469(6) 0.029(3) Uani 1 1 d . . .
O78 O -0.8186(7) 0.3652(8) -0.5534(6) 0.033(4) Uani 1 1 d . . .
O79 O -0.6823(8) 0.3638(8) -0.4435(7) 0.041(4) Uani 1 1 d . . .
O80 O -0.9378(6) 0.1432(7) -0.5692(5) 0.022(3) Uani 1 1 d U . .
N1 N -0.4683(9) 0.4642(9) -0.3826(9) 0.072(6) Uiso 1 1 d D . .
H1C H -0.4273 0.4560 -0.3876 0.107 Uiso 1 1 calc R . .
H1D H -0.4692 0.5039 -0.3651 0.107 Uiso 1 1 calc R . .
H1E H -0.4978 0.4623 -0.4225 0.107 Uiso 1 1 calc R . .
N2 N -0.5644(7) 0.4809(9) -0.2833(6) 0.041(4) Uiso 1 1 d D . .
H2C H -0.6079 0.4824 -0.2839 0.062 Uiso 1 1 calc R . .
H2D H -0.5520 0.5189 -0.2976 0.062 Uiso 1 1 calc R . .
H2E H -0.5404 0.4735 -0.2415 0.062 Uiso 1 1 calc R . .
N3 N -0.9709(9) 0.4671(10) -0.3815(9) 0.079(7) Uiso 1 1 d D . .
H3C H -0.9301 0.4594 -0.3875 0.118 Uiso 1 1 calc R . .
H3D H -0.9711 0.5057 -0.3616 0.118 Uiso 1 1 calc R . .
H3E H -1.0007 0.4674 -0.4211 0.118 Uiso 1 1 calc R . .
N4 N -1.0638(8) 0.4816(10) -0.2849(7) 0.053(4) Uiso 1 1 d D . .
H4C H -1.1072 0.4846 -0.2855 0.079 Uiso 1 1 calc R . .
H4D H -1.0503 0.5187 -0.3000 0.079 Uiso 1 1 calc R . .
H4E H -1.0400 0.4745 -0.2430 0.079 Uiso 1 1 calc R . .
N5 N -1.3018(11) 0.3398(12) -0.2085(11) 0.018(5) Uiso 0.50 1 d PD . .
N6 N -1.198(4) 0.188(3) -0.185(4) 0.19(3) Uiso 0.50 1 d PD . .
C1 C -0.4860(8) 0.4152(9) -0.3375(9) 0.043(5) Uiso 1 1 d D . .
H1A H -0.4840 0.3719 -0.3561 0.052 Uiso 1 1 calc R . .
H1B H -0.4536 0.4170 -0.2942 0.052 Uiso 1 1 calc R . .
C2 C -0.5524(7) 0.4267(8) -0.3286(7) 0.030(4) Uiso 1 1 d D . .
H2A H -0.5673 0.3863 -0.3122 0.036 Uiso 1 1 calc R . .
H2B H -0.5817 0.4346 -0.3728 0.036 Uiso 1 1 calc R . .
C3 C -0.9883(9) 0.4155(10) -0.3390(10) 0.052(5) Uiso 1 1 d D . .
H3A H -0.9875 0.3734 -0.3604 0.062 Uiso 1 1 calc R . .
H3B H -0.9553 0.4147 -0.2961 0.062 Uiso 1 1 calc R . .
C4 C -1.0537(8) 0.4266(9) -0.3282(9) 0.043(5) Uiso 1 1 d D . .
H4A H -1.0672 0.3868 -0.3095 0.051 Uiso 1 1 calc R . .
H4B H -1.0845 0.4328 -0.3719 0.051 Uiso 1 1 calc R . .
C5 C -1.2380(16) 0.3140(17) -0.173(2) 0.066(13) Uiso 0.50 1 d PD . .
H5A H -1.2049 0.3310 -0.1951 0.079 Uiso 0.50 1 calc PR . .
H5B H -1.2278 0.3329 -0.1284 0.079 Uiso 0.50 1 calc PR . .
C6 C -1.2265(19) 0.2452(16) -0.1650(19) 0.037(8) Uiso 0.50 1 d PD . .
O1W O -0.5893(8) 0.2554(9) -0.8201(8) 0.070(5) Uiso 1 1 d . . .
O2W O -0.6623(8) 0.4662(9) -0.6811(8) 0.072(5) Uiso 1 1 d . . .
O3W O -0.9225(10) 0.2422(9) -0.1970(9) 0.083(6) Uiso 1 1 d . . .
O4W O -0.7709(8) 0.1255(9) -0.1654(8) 0.074(5) Uiso 1 1 d . . .
O5W O -0.7926(12) 0.6131(13) -0.2083(12) 0.038(6) Uiso 0.50 1 d P . .
O6W O -0.9701(13) 0.0829(15) -0.3042(13) 0.051(7) Uiso 0.50 1 d P . .
O7W O -0.8421(11) 0.4728(15) -0.3216(11) 0.134(9) Uiso 1 1 d . . .
O8W O -0.6854(11) 0.2278(9) -0.2054(10) 0.084(7) Uiso 1 1 d . . .
O9W O -0.7935(11) 0.2492(12) -0.1186(11) 0.031(5) Uiso 0.50 1 d P . .
O10W O -0.9730(14) 0.5813(16) -0.3016(14) 0.169(12) Uiso 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mo1 O1 100.8(7) . . ?
O5 Mo1 O11 103.9(7) . . ?
O1 Mo1 O11 95.3(7) . . ?
O5 Mo1 O15 100.1(7) . . ?
O1 Mo1 O15 154.8(6) . . ?
O11 Mo1 O15 93.1(6) . . ?
O5 Mo1 O9 95.8(6) . . ?
O1 Mo1 O9 89.6(6) . . ?
O11 Mo1 O9 158.4(5) . . ?
O15 Mo1 O9 74.5(5) . . ?
O5 Mo1 O18 170.1(6) . . ?
O1 Mo1 O18 88.9(5) . . ?
O11 Mo1 O18 76.9(5) . . ?
O15 Mo1 O18 70.0(5) . . ?
O9 Mo1 O18 82.2(4) . . ?
O4 Mo2 O13 101.8(6) . . ?
O4 Mo2 O11 103.1(6) . . ?
O13 Mo2 O11 155.1(5) . . ?
O4 Mo2 O16 101.8(7) . . ?
O13 Mo2 O16 87.8(5) . . ?
O11 Mo2 O16 87.1(6) . . ?
O4 Mo2 O8 102.0(7) . . ?
O13 Mo2 O8 90.2(5) . . ?
O11 Mo2 O8 84.7(6) . . ?
O16 Mo2 O8 156.0(5) . . ?
O4 Mo2 O18 174.4(7) . . ?
O13 Mo2 O18 82.7(4) . . ?
O11 Mo2 O18 72.4(4) . . ?
O16 Mo2 O18 81.5(4) . . ?
O8 Mo2 O18 74.6(4) . . ?
O3 Mo3 O10 104.2(7) . . ?
O3 Mo3 O12 95.1(7) . . ?
O10 Mo3 O12 91.0(5) . . ?
O3 Mo3 O1 105.3(7) . . ?
O10 Mo3 O1 86.4(6) . . ?
O12 Mo3 O1 159.5(5) . . ?
O3 Mo3 O20 98.6(7) . . ?
O10 Mo3 O20 157.2(5) . . ?
O12 Mo3 O20 85.8(6) . . ?
O1 Mo3 O20 88.8(6) . . ?
O3 Mo3 O2 167.8(8) . . ?
O10 Mo3 O2 84.9(5) . . ?
O12 Mo3 O2 76.5(4) . . ?
O1 Mo3 O2 83.1(5) . . ?
O20 Mo3 O2 72.4(4) . . ?
O7 Mo4 O10 100.9(6) . 2_455 ?
O7 Mo4 O8 97.9(6) . . ?
O10 Mo4 O8 100.7(6) 2_455 . ?
O7 Mo4 O15 101.5(7) . . ?
O10 Mo4 O15 153.5(5) 2_455 . ?
O8 Mo4 O15 90.0(5) . . ?
O7 Mo4 O9 100.4(6) . 2_455 ?
O10 Mo4 O9 87.8(5) 2_455 2_455 ?
O8 Mo4 O9 158.0(5) . 2_455 ?
O15 Mo4 O9 74.4(5) . 2_455 ?
O7 Mo4 O18 170.2(6) . . ?
O10 Mo4 O18 88.7(5) 2_455 . ?
O8 Mo4 O18 78.3(5) . . ?
O15 Mo4 O18 69.7(5) . . ?
O9 Mo4 O18 81.7(4) 2_455 . ?
O14 Mo5 O16 106.4(6) . . ?
O14 Mo5 O20 101.6(6) . . ?
O16 Mo5 O20 97.0(6) . . ?
O14 Mo5 O17 92.9(6) . . ?
O16 Mo5 O17 155.7(5) . . ?
O20 Mo5 O17 93.3(5) . . ?
O14 Mo5 O19 96.7(6) . . ?
O16 Mo5 O19 89.3(5) . . ?
O20 Mo5 O19 158.0(5) . . ?
O17 Mo5 O19 73.5(5) . . ?
O14 Mo5 O2 167.9(6) . . ?
O16 Mo5 O2 85.6(5) . . ?
O20 Mo5 O2 75.9(5) . . ?
O17 Mo5 O2 75.6(5) . . ?
O19 Mo5 O2 83.7(4) . . ?
O6 Mo6 O13 104.7(6) . 2_455 ?
O6 Mo6 O12 100.3(6) . . ?
O13 Mo6 O12 94.8(6) 2_455 . ?
O6 Mo6 O19 97.3(6) . 2_455 ?
O13 Mo6 O19 90.6(5) 2_455 2_455 ?
O12 Mo6 O19 159.6(5) . 2_455 ?
O6 Mo6 O17 95.0(6) . . ?
O13 Mo6 O17 156.4(5) 2_455 . ?
O12 Mo6 O17 94.1(5) . . ?
O19 Mo6 O17 74.0(5) 2_455 . ?
O6 Mo6 O2 168.1(6) . . ?
O13 Mo6 O2 87.2(5) 2_455 . ?
O12 Mo6 O2 77.2(5) . . ?
O19 Mo6 O2 83.5(4) 2_455 . ?
O17 Mo6 O2 73.7(5) . . ?
O25 Mo7 O37 105.6(7) . . ?
O25 Mo7 O38 99.9(7) . . ?
O37 Mo7 O38 94.5(6) . . ?
O25 Mo7 O30 100.0(6) . . ?
O37 Mo7 O30 87.8(5) . . ?
O38 Mo7 O30 158.6(5) . . ?
O25 Mo7 O35 95.7(6) . . ?
O37 Mo7 O35 154.7(5) . . ?
O38 Mo7 O35 95.1(6) . . ?
O30 Mo7 O35 75.1(5) . . ?
O25 Mo7 O32 168.6(7) . . ?
O37 Mo7 O32 85.4(5) . . ?
O38 Mo7 O32 76.0(5) . . ?
O30 Mo7 O32 82.9(5) . . ?
O35 Mo7 O32 74.3(4) . . ?
O21 Mo8 O26 99.8(6) . . ?
O21 Mo8 O37 103.4(7) . . ?
O26 Mo8 O37 86.2(5) . . ?
O21 Mo8 O33 101.5(6) . . ?
O26 Mo8 O33 158.6(5) . . ?
O37 Mo8 O33 87.2(6) . . ?
O21 Mo8 O34 100.7(7) . . ?
O26 Mo8 O34 91.7(5) . . ?
O37 Mo8 O34 155.9(5) . . ?
O33 Mo8 O34 86.1(6) . . ?
O21 Mo8 O27 172.7(6) . . ?
O26 Mo8 O27 84.6(4) . . ?
O37 Mo8 O27 82.7(5) . . ?
O33 Mo8 O27 74.4(5) . . ?
O34 Mo8 O27 73.2(5) . . ?
O28 Mo9 O40 102.2(6) . . ?
O28 Mo9 O31 99.9(6) . . ?
O40 Mo9 O31 98.4(5) . . ?
O28 Mo9 O36 99.4(5) . . ?
O40 Mo9 O36 88.4(5) . . ?
O31 Mo9 O36 157.6(5) . . ?
O28 Mo9 O35 97.5(5) . . ?
O40 Mo9 O35 154.5(6) . . ?
O31 Mo9 O35 94.0(5) . . ?
O36 Mo9 O35 72.4(5) . . ?
O28 Mo9 O32 168.9(5) . . ?
O40 Mo9 O32 88.9(5) . . ?
O31 Mo9 O32 78.6(5) . . ?
O36 Mo9 O32 80.2(5) . . ?
O35 Mo9 O32 71.7(5) . . ?
O24 Mo10 O39 106.6(6) . . ?
O24 Mo10 O40 103.1(6) . 2_355 ?
O39 Mo10 O40 84.4(5) . 2_355 ?
O24 Mo10 O38 102.0(6) . . ?
O39 Mo10 O38 87.8(6) . . ?
O40 Mo10 O38 154.9(5) 2_355 . ?
O24 Mo10 O31 96.7(6) . . ?
O39 Mo10 O31 156.7(5) . . ?
O40 Mo10 O31 91.0(5) 2_355 . ?
O38 Mo10 O31 86.7(5) . . ?
O24 Mo10 O32 169.3(5) . . ?
O39 Mo10 O32 81.6(5) . . ?
O40 Mo10 O32 84.3(4) 2_355 . ?
O38 Mo10 O32 70.9(5) . . ?
O31 Mo10 O32 75.2(5) . . ?
O23 Mo11 O39 104.1(7) . . ?
O23 Mo11 O33 106.2(6) . . ?
O39 Mo11 O33 95.0(6) . . ?
O23 Mo11 O29 96.6(6) . 2_355 ?
O39 Mo11 O29 153.5(5) . 2_355 ?
O33 Mo11 O29 95.0(6) . 2_355 ?
O23 Mo11 O36 96.2(5) . 2_355 ?
O39 Mo11 O36 89.1(5) . 2_355 ?
O33 Mo11 O36 155.4(5) . 2_355 ?
O29 Mo11 O36 72.0(5) 2_355 2_355 ?
O23 Mo11 O27 169.4(6) . . ?
O39 Mo11 O27 86.1(5) . . ?
O33 Mo11 O27 75.4(5) . . ?
O29 Mo11 O27 72.8(5) 2_355 . ?
O36 Mo11 O27 80.7(4) 2_355 . ?
O22 Mo12 O26 102.0(6) . 2_355 ?
O22 Mo12 O34 103.2(7) . . ?
O26 Mo12 O34 98.5(5) 2_355 . ?
O22 Mo12 O30 96.7(6) . 2_355 ?
O26 Mo12 O30 87.4(5) 2_355 2_355 ?
O34 Mo12 O30 157.4(6) . 2_355 ?
O22 Mo12 O29 97.3(6) . 2_355 ?
O26 Mo12 O29 155.7(6) 2_355 2_355 ?
O34 Mo12 O29 91.1(5) . 2_355 ?
O30 Mo12 O29 75.8(5) 2_355 2_355 ?
O22 Mo12 O27 170.1(5) . . ?
O26 Mo12 O27 87.9(5) 2_355 . ?
O34 Mo12 O27 75.6(5) . . ?
O30 Mo12 O27 83.0(5) 2_355 . ?
O29 Mo12 O27 72.9(4) 2_355 . ?
O52 Mo13 O75 104.2(6) . . ?
O52 Mo13 O66 100.9(7) . . ?
O75 Mo13 O66 94.9(6) . . ?
O52 Mo13 O80 97.4(6) . . ?
O75 Mo13 O80 157.2(5) . . ?
O66 Mo13 O80 88.2(6) . . ?
O52 Mo13 O64 99.5(7) . . ?
O75 Mo13 O64 85.2(6) . . ?
O66 Mo13 O64 158.8(5) . . ?
O80 Mo13 O64 83.9(5) . . ?
O52 Mo13 O58 169.3(7) . . ?
O75 Mo13 O58 86.1(5) . . ?
O66 Mo13 O58 74.9(5) . . ?
O80 Mo13 O58 72.9(5) . . ?
O64 Mo13 O58 84.0(5) . . ?
O52 Mo13 Sb4 94.9(5) . . ?
O75 Mo13 Sb4 125.3(4) . . ?
O66 Mo13 Sb4 131.2(4) . . ?
O80 Mo13 Sb4 43.9(4) . . ?
O64 Mo13 Sb4 40.9(4) . . ?
O58 Mo13 Sb4 81.1(3) . . ?
O41 Mo14 O77 97.1(6) . . ?
O41 Mo14 O72 98.6(6) . . ?
O77 Mo14 O72 92.5(6) . . ?
O41 Mo14 O79 103.8(7) . . ?
O77 Mo14 O79 87.3(6) . . ?
O72 Mo14 O79 157.5(6) . . ?
O41 Mo14 O54 104.8(7) . . ?
O77 Mo14 O54 157.6(5) . . ?
O72 Mo14 O54 88.8(6) . . ?
O79 Mo14 O54 83.1(6) . . ?
O41 Mo14 O63 172.5(6) . . ?
O77 Mo14 O63 87.5(5) . . ?
O72 Mo14 O63 75.2(5) . . ?
O79 Mo14 O63 82.2(5) . . ?
O54 Mo14 O63 71.1(5) . . ?
O41 Mo14 Sb5 101.9(5) . . ?
O77 Mo14 Sb5 125.8(4) . . ?
O72 Mo14 Sb5 133.0(4) . . ?
O79 Mo14 Sb5 39.0(5) . . ?
O54 Mo14 Sb5 45.1(4) . . ?
O63 Mo14 Sb5 79.9(3) . . ?
O56 Mo15 O71 99.9(6) . . ?
O56 Mo15 O75 98.1(6) . . ?
O71 Mo15 O75 94.2(6) . . ?
O56 Mo15 O43 103.7(6) . . ?
O71 Mo15 O43 88.7(6) . . ?
O75 Mo15 O43 157.1(5) . . ?
O56 Mo15 O78 100.6(7) . . ?
O71 Mo15 O78 159.0(6) . . ?
O75 Mo15 O78 87.7(6) . . ?
O43 Mo15 O78 81.8(5) . . ?
O56 Mo15 O70 173.2(6) . . ?
O71 Mo15 O70 76.3(5) . . ?
O75 Mo15 O70 87.9(5) . . ?
O43 Mo15 O70 70.7(5) . . ?
O78 Mo15 O70 82.9(5) . . ?
O56 Mo15 Sb5 99.0(5) . . ?
O71 Mo15 Sb5 132.7(4) . . ?
O75 Mo15 Sb5 125.2(4) . . ?
O43 Mo15 Sb5 44.7(4) . . ?
O78 Mo15 Sb5 38.1(4) . . ?
O70 Mo15 Sb5 80.0(3) . . ?
O45 Mo16 O42 99.7(8) . . ?
O45 Mo16 O64 98.4(7) . . ?
O42 Mo16 O64 88.6(6) . . ?
O45 Mo16 O54 100.2(7) . . ?
O42 Mo16 O54 92.4(6) . . ?
O64 Mo16 O54 160.8(6) . . ?
O45 Mo16 O78 99.5(8) . . ?
O42 Mo16 O78 160.7(7) . . ?
O64 Mo16 O78 87.1(5) . . ?
O54 Mo16 O78 85.6(5) . . ?
O45 Mo16 O63 172.4(6) . . ?
O42 Mo16 O63 76.2(5) . . ?
O64 Mo16 O63 88.0(6) . . ?
O54 Mo16 O63 73.7(6) . . ?
O78 Mo16 O63 84.9(5) . . ?
O45 Mo16 Sb4 97.3(6) . . ?
O42 Mo16 Sb4 47.6(4) . . ?
O64 Mo16 Sb4 41.5(4) . . ?
O54 Mo16 Sb4 138.7(4) . . ?
O78 Mo16 Sb4 127.8(4) . . ?
O63 Mo16 Sb4 84.8(3) . . ?
O45 Mo16 Sb5 96.8(6) . . ?
O42 Mo16 Sb5 138.3(4) . . ?
O64 Mo16 Sb5 126.3(3) . . ?
O54 Mo16 Sb5 46.9(4) . . ?
O78 Mo16 Sb5 39.6(4) . . ?
O63 Mo16 Sb5 82.5(3) . . ?
Sb4 Mo16 Sb5 162.83(10) . . ?
O50 Mo17 O53 102.0(7) . . ?
O50 Mo17 O44 100.9(7) . 4_344 ?
O53 Mo17 O44 90.5(6) . 4_344 ?
O50 Mo17 O65 100.9(6) . . ?
O53 Mo17 O65 83.2(6) . . ?
O44 Mo17 O65 158.1(6) 4_344 . ?
O50 Mo17 O73 96.5(6) . 4_344 ?
O53 Mo17 O73 161.5(6) . 4_344 ?
O44 Mo17 O73 84.4(6) 4_344 4_344 ?
O65 Mo17 O73 95.0(5) . 4_344 ?
O50 Mo17 O62 170.5(6) . . ?
O53 Mo17 O62 85.3(6) . . ?
O44 Mo17 O62 84.9(5) 4_344 . ?
O65 Mo17 O62 73.7(5) . . ?
O73 Mo17 O62 76.5(5) 4_344 . ?
O50 Mo17 Sb6 96.1(5) . 4_344 ?
O53 Mo17 Sb6 129.9(4) . 4_344 ?
O44 Mo17 Sb6 40.0(5) 4_344 4_344 ?
O65 Mo17 Sb6 138.2(4) . 4_344 ?
O73 Mo17 Sb6 45.0(3) 4_344 4_344 ?
O62 Mo17 Sb6 83.5(3) . 4_344 ?
O50 Mo17 Sb3 99.1(5) . . ?
O53 Mo17 Sb3 38.4(4) . . ?
O44 Mo17 Sb3 128.1(5) 4_344 . ?
O65 Mo17 Sb3 45.6(4) . . ?
O73 Mo17 Sb3 139.6(4) 4_344 . ?
O62 Mo17 Sb3 82.8(3) . . ?
Sb6 Mo17 Sb3 162.84(10) 4_344 . ?
O46 Mo18 O80 99.6(6) . . ?
O46 Mo18 O61 96.1(7) . 4_344 ?
O80 Mo18 O61 95.8(5) . 4_344 ?
O46 Mo18 O74 102.9(7) . . ?
O80 Mo18 O74 81.8(5) . . ?
O61 Mo18 O74 161.0(6) 4_344 . ?
O46 Mo18 O59 103.4(7) . 4_344 ?
O80 Mo18 O59 156.6(7) . 4_344 ?
O61 Mo18 O59 86.1(6) 4_344 4_344 ?
O74 Mo18 O59 88.9(6) . 4_344 ?
O46 Mo18 O58 169.8(6) . . ?
O80 Mo18 O58 73.6(5) . . ?
O61 Mo18 O58 77.4(6) 4_344 . ?
O74 Mo18 O58 83.9(6) . . ?
O59 Mo18 O58 84.1(6) 4_344 . ?
O46 Mo18 Sb6 96.5(5) . 4_344 ?
O80 Mo18 Sb6 139.9(4) . 4_344 ?
O61 Mo18 Sb6 45.9(4) 4_344 4_344 ?
O74 Mo18 Sb6 129.6(4) . 4_344 ?
O59 Mo18 Sb6 41.1(5) 4_344 4_344 ?
O58 Mo18 Sb6 84.5(4) . 4_344 ?
O46 Mo18 Sb4 99.4(5) . . ?
O80 Mo18 Sb4 44.3(4) . . ?
O61 Mo18 Sb4 138.9(4) 4_344 . ?
O74 Mo18 Sb4 38.2(4) . . ?
O59 Mo18 Sb4 126.0(5) 4_344 . ?
O58 Mo18 Sb4 81.2(4) . . ?
Sb6 Mo18 Sb4 162.15(10) 4_344 . ?
O57 Mo19 O60 99.4(7) . . ?
O57 Mo19 O43 102.0(7) . . ?
O60 Mo19 O43 93.4(6) . . ?
O57 Mo19 O79 101.3(7) . . ?
O60 Mo19 O79 159.0(6) . . ?
O43 Mo19 O79 85.8(6) . . ?
O57 Mo19 O68 97.4(6) . . ?
O60 Mo19 O68 88.7(6) . . ?
O43 Mo19 O68 159.9(6) . . ?
O79 Mo19 O68 85.2(6) . . ?
O57 Mo19 O70 172.9(6) . . ?
O60 Mo19 O70 75.5(5) . . ?
O43 Mo19 O70 73.6(6) . . ?
O79 Mo19 O70 84.2(5) . . ?
O68 Mo19 O70 87.6(5) . . ?
O57 Mo19 Sb5 98.7(5) . . ?
O60 Mo19 Sb5 138.3(4) . . ?
O43 Mo19 Sb5 46.0(4) . . ?
O79 Mo19 Sb5 40.7(5) . . ?
O68 Mo19 Sb5 125.6(4) . . ?
O70 Mo19 Sb5 82.3(3) . . ?
O57 Mo19 Sb3 95.5(5) . . ?
O60 Mo19 Sb3 46.9(4) . . ?
O43 Mo19 Sb3 139.0(5) . . ?
O79 Mo19 Sb3 126.8(5) . . ?
O68 Mo19 Sb3 42.4(4) . . ?
O70 Mo19 Sb3 84.8(3) . . ?
Sb5 Mo19 Sb3 163.00(10) . . ?
O51 Mo20 O77 103.5(7) . . ?
O51 Mo20 O69 99.3(7) . . ?
O77 Mo20 O69 94.8(6) . . ?
O51 Mo20 O68 100.8(7) . . ?
O77 Mo20 O68 85.6(6) . . ?
O69 Mo20 O68 159.2(5) . . ?
O51 Mo20 O65 99.4(6) . . ?
O77 Mo20 O65 156.4(5) . . ?
O69 Mo20 O65 86.7(5) . . ?
O68 Mo20 O65 84.8(5) . . ?
O51 Mo20 O62 169.1(7) . . ?
O77 Mo20 O62 86.1(5) . . ?
O69 Mo20 O62 74.4(5) . . ?
O68 Mo20 O62 84.9(5) . . ?
O65 Mo20 O62 71.7(4) . . ?
O51 Mo20 Sb3 96.5(5) . . ?
O77 Mo20 Sb3 126.0(4) . . ?
O69 Mo20 Sb3 130.8(4) . . ?
O68 Mo20 Sb3 41.2(4) . . ?
O65 Mo20 Sb3 44.7(4) . . ?
O62 Mo20 Sb3 81.7(3) . . ?
O49 Mo21 O76 99.9(6) . . ?
O49 Mo21 O71 101.5(6) . . ?
O76 Mo21 O71 93.0(6) . . ?
O49 Mo21 O60 104.0(6) . . ?
O76 Mo21 O60 155.4(5) . . ?
O71 Mo21 O60 88.2(6) . . ?
O49 Mo21 O53 100.5(6) . . ?
O76 Mo21 O53 87.9(5) . . ?
O71 Mo21 O53 157.4(6) . . ?
O60 Mo21 O53 81.8(6) . . ?
O49 Mo21 O70 172.9(6) . . ?
O76 Mo21 O70 86.3(5) . . ?
O71 Mo21 O70 74.5(5) . . ?
O60 Mo21 O70 70.3(5) . . ?
O53 Mo21 O70 83.1(5) . . ?
O49 Mo21 Sb3 98.0(4) . . ?
O76 Mo21 Sb3 125.1(4) . . ?
O71 Mo21 Sb3 132.9(4) . . ?
O60 Mo21 Sb3 45.4(4) . . ?
O53 Mo21 Sb3 37.8(4) . . ?
O70 Mo21 Sb3 81.0(3) . . ?
O47 Mo22 O67 99.5(6) . . ?
O47 Mo22 O72 99.9(6) . . ?
O67 Mo22 O72 91.8(6) . . ?
O47 Mo22 O42 104.8(6) . . ?
O67 Mo22 O42 155.2(6) . . ?
O72 Mo22 O42 88.7(6) . . ?
O47 Mo22 O74 101.7(6) . . ?
O67 Mo22 O74 88.5(6) . . ?
O72 Mo22 O74 158.0(6) . . ?
O42 Mo22 O74 81.9(6) . . ?
O47 Mo22 O63 173.1(6) . . ?
O67 Mo22 O63 85.1(5) . . ?
O72 Mo22 O63 74.7(5) . . ?
O42 Mo22 O63 71.2(5) . . ?
O74 Mo22 O63 83.4(5) . . ?
O47 Mo22 Sb4 100.2(4) . . ?
O67 Mo22 Sb4 125.0(4) . . ?
O72 Mo22 Sb4 133.7(4) . . ?
O42 Mo22 Sb4 45.8(4) . . ?
O74 Mo22 Sb4 37.2(4) . . ?
O63 Mo22 Sb4 81.1(3) . . ?
O48 Mo23 O66 97.9(7) . . ?
O48 Mo23 O76 104.1(6) . . ?
O66 Mo23 O76 96.3(5) . . ?
O48 Mo23 O44 103.6(7) . 4_344 ?
O66 Mo23 O44 157.5(5) . 4_344 ?
O76 Mo23 O44 84.8(5) . 4_344 ?
O48 Mo23 O61 96.3(7) . 4_344 ?
O66 Mo23 O61 88.4(5) . 4_344 ?
O76 Mo23 O61 158.2(5) . 4_344 ?
O44 Mo23 O61 82.9(6) 4_344 4_344 ?
O48 Mo23 O58 167.9(6) . . ?
O66 Mo23 O58 73.8(5) . . ?
O76 Mo23 O58 85.9(5) . . ?
O44 Mo23 O58 83.9(5) 4_344 . ?
O61 Mo23 O58 75.0(6) 4_344 . ?
O48 Mo23 Sb6 97.1(6) . 4_344 ?
O66 Mo23 Sb6 131.8(4) . 4_344 ?
O76 Mo23 Sb6 123.7(3) . 4_344 ?
O44 Mo23 Sb6 39.3(4) 4_344 4_344 ?
O61 Mo23 Sb6 44.5(4) 4_344 4_344 ?
O58 Mo23 Sb6 82.7(4) . 4_344 ?
O55 Mo24 O67 105.3(6) . . ?
O55 Mo24 O69 98.7(6) . . ?
O67 Mo24 O69 96.2(6) . . ?
O55 Mo24 O59 103.4(7) . 4_344 ?
O67 Mo24 O59 84.9(6) . 4_344 ?
O69 Mo24 O59 156.8(6) . 4_344 ?
O55 Mo24 O73 95.6(6) . 4_344 ?
O67 Mo24 O73 157.4(5) . 4_344 ?
O69 Mo24 O73 88.8(5) . 4_344 ?
O59 Mo24 O73 82.1(6) 4_344 4_344 ?
O55 Mo24 O62 168.3(6) . . ?
O67 Mo24 O62 85.1(6) . . ?
O69 Mo24 O62 74.5(4) . . ?
O59 Mo24 O62 82.6(6) 4_344 . ?
O73 Mo24 O62 75.0(5) 4_344 . ?
O55 Mo24 Sb6 95.9(5) . 4_344 ?
O67 Mo24 Sb6 123.8(4) . 4_344 ?
O69 Mo24 Sb6 131.5(3) . 4_344 ?
O59 Mo24 Sb6 39.3(5) 4_344 4_344 ?
O73 Mo24 Sb6 43.8(3) 4_344 4_344 ?
O62 Mo24 Sb6 82.2(3) . 4_344 ?
O19 Sb1 O19 98.3(7) . 2_455 ?
O19 Sb1 O17 73.6(5) . . ?
O19 Sb1 O17 76.9(5) 2_455 . ?
O19 Sb1 O17 76.9(5) . 2_455 ?
O19 Sb1 O17 73.6(5) 2_455 2_455 ?
O17 Sb1 O17 134.2(8) . 2_455 ?
O36 Sb2 O30 96.8(5) . . ?
O36 Sb2 O35 75.5(5) . . ?
O30 Sb2 O35 72.1(5) . . ?
O36 Sb2 O29 72.5(5) . . ?
O30 Sb2 O29 76.3(5) . . ?
O35 Sb2 O29 131.3(5) . . ?
Sb3 Sb3 O53 131.6(5) 2_454 . ?
Sb3 Sb3 O68 129.9(4) 2_454 . ?
O53 Sb3 O68 98.4(5) . . ?
Sb3 Sb3 O65 114.4(3) 2_454 . ?
O53 Sb3 O65 70.7(5) . . ?
O68 Sb3 O65 75.1(5) . . ?
Sb3 Sb3 O60 116.0(4) 2_454 . ?
O53 Sb3 O60 75.9(6) . . ?
O68 Sb3 O60 73.8(5) . . ?
O65 Sb3 O60 129.6(5) . . ?
Sb3 Sb3 Mo17 126.66(6) 2_454 . ?
O53 Sb3 Mo17 34.8(4) . . ?
O68 Sb3 Mo17 91.1(4) . . ?
O65 Sb3 Mo17 36.5(3) . . ?
O60 Sb3 Mo17 106.4(4) . . ?
Sb3 Sb3 Mo19 127.46(7) 2_454 . ?
O53 Sb3 Mo19 90.7(5) . . ?
O68 Sb3 Mo19 38.3(4) . . ?
O65 Sb3 Mo19 107.7(3) . . ?
O60 Sb3 Mo19 36.1(3) . . ?
Mo17 Sb3 Mo19 105.88(9) . . ?
Sb3 Sb3 Mo20 125.9(2) 2_454 . ?
O53 Sb3 Mo20 89.4(4) . . ?
O68 Sb3 Mo20 36.8(4) . . ?
O65 Sb3 Mo20 39.1(3) . . ?
O60 Sb3 Mo20 106.0(3) . . ?
Mo17 Sb3 Mo20 65.23(7) . . ?
Mo19 Sb3 Mo20 73.50(8) . . ?
Sb3 Sb3 Mo21 127.1(2) 2_454 . ?
O53 Sb3 Mo21 38.9(4) . . ?
O68 Sb3 Mo21 92.0(3) . . ?
O65 Sb3 Mo21 105.8(3) . . ?
O60 Sb3 Mo21 38.2(4) . . ?
Mo17 Sb3 Mo21 72.71(8) . . ?
Mo19 Sb3 Mo21 64.25(7) . . ?
Mo20 Sb3 Mo21 106.94(9) . . ?
Sb4 Sb4 O74 133.2(5) 2_354 . ?
Sb4 Sb4 O64 127.7(4) 2_354 . ?
O74 Sb4 O64 99.1(6) . . ?
Sb4 Sb4 O80 111.7(3) 2_354 . ?
O74 Sb4 O80 73.0(5) . . ?
O64 Sb4 O80 77.9(5) . . ?
Sb4 Sb4 O42 116.3(4) 2_354 . ?
O74 Sb4 O42 75.2(6) . . ?
O64 Sb4 O42 72.6(5) . . ?
O80 Sb4 O42 132.0(5) . . ?
Sb4 Sb4 Mo16 126.87(7) 2_354 . ?
O74 Sb4 Mo16 90.3(5) . . ?
O64 Sb4 Mo16 36.6(4) . . ?
O80 Sb4 Mo16 109.2(3) . . ?
O42 Sb4 Mo16 36.4(3) . . ?
Sb4 Sb4 Mo18 126.54(7) 2_354 . ?
O74 Sb4 Mo18 36.4(4) . . ?
O64 Sb4 Mo18 92.9(4) . . ?
O80 Sb4 Mo18 37.2(3) . . ?
O42 Sb4 Mo18 107.5(4) . . ?
Mo16 Sb4 Mo18 106.54(9) . . ?
Sb4 Sb4 Mo13 123.5(2) 2_354 . ?
O74 Sb4 Mo13 90.6(4) . . ?
O64 Sb4 Mo13 39.1(4) . . ?
O80 Sb4 Mo13 39.5(3) . . ?
O42 Sb4 Mo13 107.1(3) . . ?
Mo16 Sb4 Mo13 74.05(8) . . ?
Mo18 Sb4 Mo13 65.33(8) . . ?
Sb4 Sb4 Mo22 129.2(2) 2_354 . ?
O74 Sb4 Mo22 37.5(4) . . ?
O64 Sb4 Mo22 91.2(3) . . ?
O80 Sb4 Mo22 107.0(3) . . ?
O42 Sb4 Mo22 38.8(3) . . ?
Mo16 Sb4 Mo22 64.52(7) . . ?
Mo18 Sb4 Mo22 72.83(8) . . ?
Mo13 Sb4 Mo22 107.31(9) . . ?
Sb6 Sb5 O78 129.9(5) . . ?
Sb6 Sb5 O79 132.3(5) . . ?
O78 Sb5 O79 97.7(8) . . ?
Sb6 Sb5 O43 114.1(4) . . ?
O78 Sb5 O43 74.6(5) . . ?
O79 Sb5 O43 73.8(5) . . ?
Sb6 Sb5 O54 115.8(4) . . ?
O78 Sb5 O54 73.7(5) . . ?
O79 Sb5 O54 73.5(5) . . ?
O43 Sb5 O54 130.1(7) . . ?
Sb6 Sb5 Mo16 127.05(18) . . ?
O78 Sb5 Mo16 37.2(4) . . ?
O79 Sb5 Mo16 89.7(4) . . ?
O43 Sb5 Mo16 107.0(4) . . ?
O54 Sb5 Mo16 37.2(3) . . ?
Sb6 Sb5 Mo19 126.81(18) . . ?
O78 Sb5 Mo19 90.7(5) . . ?
O79 Sb5 Mo19 37.7(4) . . ?
O43 Sb5 Mo19 36.9(3) . . ?
O54 Sb5 Mo19 106.8(4) . . ?
Mo16 Sb5 Mo19 106.12(11) . . ?
Sb6 Sb5 Mo15 125.39(19) . . ?
O78 Sb5 Mo15 37.4(4) . . ?
O79 Sb5 Mo15 90.7(4) . . ?
O43 Sb5 Mo15 38.1(3) . . ?
O54 Sb5 Mo15 106.7(4) . . ?
Mo16 Sb5 Mo15 73.28(8) . . ?
Mo19 Sb5 Mo15 64.62(7) . . ?
Sb6 Sb5 Mo14 127.97(19) . . ?
O78 Sb5 Mo14 90.9(4) . . ?
O79 Sb5 Mo14 36.4(4) . . ?
O43 Sb5 Mo14 106.2(4) . . ?
O54 Sb5 Mo14 38.0(3) . . ?
Mo16 Sb5 Mo14 64.66(8) . . ?
Mo19 Sb5 Mo14 73.04(8) . . ?
Mo15 Sb5 Mo14 106.64(12) . . ?
Sb5 Sb6 O44 131.4(5) . . ?
Sb5 Sb6 O59 133.8(5) . . ?
O44 Sb6 O59 94.8(8) . . ?
Sb5 Sb6 O73 113.5(4) . . ?
O44 Sb6 O73 73.1(5) . . ?
O59 Sb6 O73 75.0(6) . . ?
Sb5 Sb6 O61 110.5(4) . . ?
O44 Sb6 O61 77.8(6) . . ?
O59 Sb6 O61 75.3(6) . . ?
O73 Sb6 O61 136.0(6) . . ?
Sb5 Sb6 Mo18 125.59(18) . 4_354 ?
O44 Sb6 Mo18 91.0(5) . 4_354 ?
O59 Sb6 Mo18 38.2(4) . 4_354 ?
O73 Sb6 Mo18 110.2(4) . 4_354 ?
O61 Sb6 Mo18 37.8(3) . 4_354 ?
Sb5 Sb6 Mo17 127.09(18) . 4_354 ?
O44 Sb6 Mo17 35.6(4) . 4_354 ?
O59 Sb6 Mo17 88.7(5) . 4_354 ?
O73 Sb6 Mo17 38.0(3) . 4_354 ?
O61 Sb6 Mo17 110.1(4) . 4_354 ?
Mo18 Sb6 Mo17 107.28(12) 4_354 4_354 ?
Sb5 Sb6 Mo24 128.13(19) . 4_354 ?
O44 Sb6 Mo24 88.9(4) . 4_354 ?
O59 Sb6 Mo24 36.3(4) . 4_354 ?
O73 Sb6 Mo24 39.6(3) . 4_354 ?
O61 Sb6 Mo24 108.9(4) . 4_354 ?
Mo18 Sb6 Mo24 73.90(8) 4_354 4_354 ?
Mo17 Sb6 Mo24 64.72(7) 4_354 4_354 ?
Sb5 Sb6 Mo23 125.01(19) . 4_354 ?
O44 Sb6 Mo23 38.9(4) . 4_354 ?
O59 Sb6 Mo23 89.6(5) . 4_354 ?
O73 Sb6 Mo23 108.9(3) . 4_354 ?
O61 Sb6 Mo23 39.7(4) . 4_354 ?
Mo18 Sb6 Mo23 64.63(8) 4_354 4_354 ?
Mo17 Sb6 Mo23 73.73(8) 4_354 4_354 ?
Mo24 Sb6 Mo23 106.85(12) 4_354 4_354 ?
O9 Sb7 O9 99.4(7) . 2_455 ?
O9 Sb7 O15 72.6(5) . . ?
O9 Sb7 O15 73.1(5) 2_455 . ?
O9 Sb7 O15 73.1(5) . 2_455 ?
O9 Sb7 O15 72.6(5) 2_455 2_455 ?
O15 Sb7 O15 125.8(8) . 2_455 ?
O2 Si1 O2 115.9(11) . 2_455 ?
O2 Si1 O18 109.3(5) . 2_455 ?
O2 Si1 O18 108.3(5) 2_455 2_455 ?
O2 Si1 O18 108.3(5) . . ?
O2 Si1 O18 109.3(5) 2_455 . ?
O18 Si1 O18 105.2(10) 2_455 . ?
O32 Si2 O32 114.7(12) 2_355 . ?
O32 Si2 O27 109.3(6) 2_355 2_355 ?
O32 Si2 O27 109.4(6) . 2_355 ?
O32 Si2 O27 109.4(6) 2_355 . ?
O32 Si2 O27 109.3(5) . . ?
O27 Si2 O27 104.1(10) 2_355 . ?
O62 Si3 O58 115.3(10) . . ?
O62 Si3 O70 110.2(6) . . ?
O58 Si3 O70 109.1(6) . . ?
O62 Si3 O63 109.1(6) . . ?
O58 Si3 O63 108.1(6) . . ?
O70 Si3 O63 104.4(9) . . ?
Mo1 O1 Mo3 151.8(7) . . ?
Si1 O2 Mo5 123.6(6) . . ?
Si1 O2 Mo6 122.3(6) . . ?
Mo5 O2 Mo6 95.1(5) . . ?
Si1 O2 Mo3 128.2(8) . . ?
Mo5 O2 Mo3 89.5(4) . . ?
Mo6 O2 Mo3 88.0(4) . . ?
Mo4 O8 Mo2 119.5(6) . . ?
Sb7 O9 Mo1 108.1(5) . . ?
Sb7 O9 Mo4 107.0(5) . 2_455 ?
Mo1 O9 Mo4 138.8(7) . 2_455 ?
Mo4 O10 Mo3 154.4(7) 2_455 . ?
Mo1 O11 Mo2 123.4(7) . . ?
Mo6 O12 Mo3 118.1(6) . . ?
Mo6 O13 Mo2 152.5(7) 2_455 . ?
Mo4 O15 Mo1 120.9(7) . . ?
Mo4 O15 Sb7 103.5(5) . . ?
Mo1 O15 Sb7 103.0(5) . . ?
Mo5 O16 Mo2 155.7(6) . . ?
Mo5 O17 Sb1 103.4(5) . . ?
Mo5 O17 Mo6 112.7(7) . . ?
Sb1 O17 Mo6 100.7(5) . . ?
Si1 O18 Mo1 126.6(6) . . ?
Si1 O18 Mo4 126.1(5) . . ?
Mo1 O18 Mo4 95.6(4) . . ?
Si1 O18 Mo2 122.4(7) . . ?
Mo1 O18 Mo2 87.3(3) . . ?
Mo4 O18 Mo2 86.9(3) . . ?
Sb1 O19 Mo5 108.8(5) . . ?
Sb1 O19 Mo6 107.3(5) . 2_455 ?
Mo5 O19 Mo6 138.4(7) . 2_455 ?
Mo5 O20 Mo3 122.1(6) . . ?
Mo12 O26 Mo8 152.5(8) 2_355 . ?
Si2 O27 Mo12 126.7(6) . . ?
Si2 O27 Mo8 126.4(6) . . ?
Mo12 O27 Mo8 88.7(4) . . ?
Si2 O27 Mo11 121.9(7) . . ?
Mo12 O27 Mo11 94.8(4) . . ?
Mo8 O27 Mo11 87.4(3) . . ?
Mo11 O29 Mo12 116.1(6) 2_355 2_355 ?
Mo11 O29 Sb2 103.7(7) 2_355 . ?
Mo12 O29 Sb2 101.6(5) 2_355 . ?
Mo7 O30 Sb2 107.8(7) . . ?
Mo7 O30 Mo12 141.0(6) . 2_355 ?
Sb2 O30 Mo12 104.8(5) . 2_355 ?
Mo9 O31 Mo10 119.0(6) . . ?
Si2 O32 Mo7 128.3(8) . . ?
Si2 O32 Mo9 123.1(6) . . ?
Mo7 O32 Mo9 95.7(4) . . ?
Si2 O32 Mo10 122.7(6) . . ?
Mo7 O32 Mo10 88.7(4) . . ?
Mo9 O32 Mo10 86.9(5) . . ?
Mo11 O33 Mo8 122.8(7) . . ?
Mo12 O34 Mo8 122.2(7) . . ?
Mo7 O35 Mo9 114.5(5) . . ?
Mo7 O35 Sb2 104.3(7) . . ?
Mo9 O35 Sb2 101.5(5) . . ?
Sb2 O36 Mo11 110.0(7) . 2_355 ?
Sb2 O36 Mo9 108.7(5) . . ?
Mo11 O36 Mo9 138.3(6) 2_355 . ?
Mo7 O37 Mo8 155.4(7) . . ?
Mo7 O38 Mo10 124.4(7) . . ?
Mo11 O39 Mo10 156.9(6) . . ?
Mo9 O40 Mo10 156.2(8) . 2_355 ?
Mo16 O42 Mo22 121.0(7) . . ?
Mo16 O42 Sb4 95.9(5) . . ?
Mo22 O42 Sb4 95.4(6) . . ?
Mo19 O43 Mo15 121.3(8) . . ?
Mo19 O43 Sb5 97.1(5) . . ?
Mo15 O43 Sb5 97.2(5) . . ?
Mo17 O44 Mo23 149.5(9) 4_354 4_354 ?
Mo17 O44 Sb6 104.4(7) 4_354 . ?
Mo23 O44 Sb6 101.8(7) 4_354 . ?
Mo17 O53 Sb3 106.7(6) . . ?
Mo17 O53 Mo21 145.2(7) . . ?
Sb3 O53 Mo21 103.4(7) . . ?
Mo16 O54 Mo14 121.3(8) . . ?
Mo16 O54 Sb5 96.0(5) . . ?
Mo14 O54 Sb5 96.9(5) . . ?
Si3 O58 Mo13 128.8(9) . . ?
Si3 O58 Mo18 122.2(7) . . ?
Mo13 O58 Mo18 93.5(5) . . ?
Si3 O58 Mo23 121.6(7) . . ?
Mo13 O58 Mo23 89.6(4) . . ?
Mo18 O58 Mo23 91.1(6) . . ?
Mo24 O59 Mo18 151.8(10) 4_354 4_354 ?
Mo24 O59 Sb6 104.5(7) 4_354 . ?
Mo18 O59 Sb6 100.7(7) 4_354 . ?
Mo19 O60 Mo21 122.0(7) . . ?
Mo19 O60 Sb3 97.0(5) . . ?
Mo21 O60 Sb3 96.4(6) . . ?
Mo18 O61 Mo23 116.2(7) 4_354 4_354 ?
Mo18 O61 Sb6 96.2(5) 4_354 . ?
Mo23 O61 Sb6 95.8(5) 4_354 . ?
Si3 O62 Mo24 123.9(6) . . ?
Si3 O62 Mo20 126.9(8) . . ?
Mo24 O62 Mo20 89.4(4) . . ?
Si3 O62 Mo17 122.1(6) . . ?
Mo24 O62 Mo17 92.0(5) . . ?
Mo20 O62 Mo17 92.7(4) . . ?
Si3 O63 Mo16 126.6(6) . . ?
Si3 O63 Mo14 125.2(6) . . ?
Mo16 O63 Mo14 93.3(5) . . ?
Si3 O63 Mo22 121.3(8) . . ?
Mo16 O63 Mo22 91.4(4) . . ?
Mo14 O63 Mo22 88.6(4) . . ?
Mo16 O64 Mo13 148.9(6) . . ?
Mo16 O64 Sb4 101.9(5) . . ?
Mo13 O64 Sb4 100.0(6) . . ?
Mo17 O65 Mo20 121.5(6) . . ?
Mo17 O65 Sb3 97.9(5) . . ?
Mo20 O65 Sb3 96.2(6) . . ?
Mo23 O66 Mo13 121.3(6) . . ?
Mo22 O67 Mo24 155.8(7) . . ?
Mo20 O68 Mo19 149.5(7) . . ?
Mo20 O68 Sb3 102.1(7) . . ?
Mo19 O68 Sb3 99.3(5) . . ?
Mo20 O69 Mo24 121.2(5) . . ?
Si3 O70 Mo19 126.5(6) . . ?
Si3 O70 Mo15 125.3(6) . . ?
Mo19 O70 Mo15 93.7(5) . . ?
Si3 O70 Mo21 120.8(7) . . ?
Mo19 O70 Mo21 91.8(4) . . ?
Mo15 O70 Mo21 88.4(4) . . ?
Mo15 O71 Mo21 120.5(6) . . ?
Mo22 O72 Mo14 121.3(6) . . ?
Mo17 O73 Mo24 116.0(7) 4_354 4_354 ?
Mo17 O73 Sb6 97.0(5) 4_354 . ?
Mo24 O73 Sb6 96.6(5) 4_354 . ?
Mo18 O74 Sb4 105.4(6) . . ?
Mo18 O74 Mo22 144.7(7) . . ?
Sb4 O74 Mo22 105.4(8) . . ?
Mo13 O75 Mo15 153.1(7) . . ?
Mo21 O76 Mo23 154.9(6) . . ?
Mo20 O77 Mo14 152.4(7) . . ?
Mo16 O78 Mo15 146.0(9) . . ?
Mo16 O78 Sb5 103.3(6) . . ?
Mo15 O78 Sb5 104.5(6) . . ?
Mo19 O79 Mo14 148.3(10) . . ?
Mo19 O79 Sb5 101.6(7) . . ?
Mo14 O79 Sb5 104.6(7) . . ?
Mo18 O80 Mo13 119.1(6) . . ?
Mo18 O80 Sb4 98.6(4) . . ?
Mo13 O80 Sb4 96.6(6) . . ?
C2 C1 N1 111.0(15) . . ?
C1 C2 N2 120.3(14) . . ?
C4 C3 N3 110.8(17) . . ?
C3 C4 N4 119.4(16) . . ?
C6 C5 N5 122(3) . . ?
N6 C6 C5 148(5) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O5 1.687(16) . ?
Mo1 O1 1.806(14) . ?
Mo1 O11 1.856(14) . ?
Mo1 O15 2.029(12) . ?
Mo1 O9 2.067(12) . ?
Mo1 O18 2.368(11) . ?
Mo2 O4 1.621(14) . ?
Mo2 O13 1.943(12) . ?
Mo2 O11 1.949(17) . ?
Mo2 O16 1.956(13) . ?
Mo2 O8 1.979(14) . ?
Mo2 O18 2.487(11) . ?
Mo3 O3 1.633(11) . ?
Mo3 O10 1.876(12) . ?
Mo3 O12 1.959(14) . ?
Mo3 O1 1.986(13) . ?
Mo3 O20 2.006(15) . ?
Mo3 O2 2.403(12) . ?
Mo4 O7 1.653(15) . ?
Mo4 O10 1.861(12) 2_455 ?
Mo4 O8 1.904(12) . ?
Mo4 O15 2.023(14) . ?
Mo4 O9 2.102(12) 2_455 ?
Mo4 O18 2.388(11) . ?
Mo5 O14 1.752(16) . ?
Mo5 O16 1.800(12) . ?
Mo5 O20 1.836(13) . ?
Mo5 O17 2.069(14) . ?
Mo5 O19 2.070(11) . ?
Mo5 O2 2.376(13) . ?
Mo6 O6 1.696(15) . ?
Mo6 O13 1.820(13) 2_455 ?
Mo6 O12 1.929(12) . ?
Mo6 O19 2.116(11) 2_455 ?
Mo6 O17 2.158(14) . ?
Mo6 O2 2.395(12) . ?
Mo7 O25 1.666(10) . ?
Mo7 O37 1.838(14) . ?
Mo7 O38 1.848(15) . ?
Mo7 O30 2.011(13) . ?
Mo7 O35 2.043(14) . ?
Mo7 O32 2.339(12) . ?
Mo8 O21 1.633(17) . ?
Mo8 O26 1.922(11) . ?
Mo8 O37 1.922(14) . ?
Mo8 O33 1.952(15) . ?
Mo8 O34 1.955(13) . ?
Mo8 O27 2.421(12) . ?
Mo9 O28 1.702(13) . ?
Mo9 O40 1.798(11) . ?
Mo9 O31 1.906(13) . ?
Mo9 O36 2.106(13) . ?
Mo9 O35 2.128(13) . ?
Mo9 O32 2.392(12) . ?
Mo10 O24 1.724(13) . ?
Mo10 O39 1.924(14) . ?
Mo10 O40 1.941(11) 2_355 ?
Mo10 O38 1.960(14) . ?
Mo10 O31 1.982(13) . ?
Mo10 O32 2.478(13) . ?
Mo11 O23 1.671(11) . ?
Mo11 O39 1.821(14) . ?
Mo11 O33 1.868(15) . ?
Mo11 O29 2.051(14) 2_355 ?
Mo11 O36 2.077(12) 2_355 ?
Mo11 O27 2.438(11) . ?
Mo12 O22 1.691(14) . ?
Mo12 O26 1.836(12) 2_355 ?
Mo12 O34 1.876(12) . ?
Mo12 O30 2.111(13) 2_355 ?
Mo12 O29 2.125(14) 2_355 ?
Mo12 O27 2.376(12) . ?
Mo13 O52 1.716(12) . ?
Mo13 O75 1.862(14) . ?
Mo13 O66 1.911(13) . ?
Mo13 O80 2.046(13) . ?
Mo13 O64 2.046(14) . ?
Mo13 O58 2.327(13) . ?
Mo13 Sb4 3.193(3) . ?
Mo14 O41 1.637(13) . ?
Mo14 O77 1.924(15) . ?
Mo14 O72 1.945(14) . ?
Mo14 O79 1.982(15) . ?
Mo14 O54 2.002(13) . ?
Mo14 O63 2.367(13) . ?
Mo14 Sb5 3.231(3) . ?
Mo15 O56 1.624(14) . ?
Mo15 O71 1.920(13) . ?
Mo15 O75 1.922(13) . ?
Mo15 O43 2.005(14) . ?
Mo15 O78 2.025(14) . ?
Mo15 O70 2.366(12) . ?
Mo15 Sb5 3.227(3) . ?
Mo16 O45 1.627(16) . ?
Mo16 O42 1.871(14) . ?
Mo16 O64 1.909(14) . ?
Mo16 O54 1.909(13) . ?
Mo16 O78 1.952(14) . ?
Mo16 O63 2.323(13) . ?
Mo16 Sb4 3.133(4) . ?
Mo16 Sb5 3.144(3) . ?
Mo17 O50 1.666(15) . ?
Mo17 O53 1.876(15) . ?
Mo17 O44 1.889(14) 4_344 ?
Mo17 O65 1.889(12) . ?
Mo17 O73 1.949(13) 4_344 ?
Mo17 O62 2.375(14) . ?
Mo17 Sb6 3.140(3) 4_344 ?
Mo17 Sb3 3.146(4) . ?
Mo18 O46 1.696(15) . ?
Mo18 O80 1.929(12) . ?
Mo18 O61 1.937(14) 4_344 ?
Mo18 O74 1.942(16) . ?
Mo18 O59 1.975(16) 4_344 ?
Mo18 O58 2.379(16) . ?
Mo18 Sb6 3.138(3) 4_344 ?
Mo18 Sb4 3.157(4) . ?
Mo19 O57 1.716(14) . ?
Mo19 O60 1.873(14) . ?
Mo19 O43 1.908(12) . ?
Mo19 O79 1.970(15) . ?
Mo19 O68 1.984(14) . ?
Mo19 O70 2.311(13) . ?
Mo19 Sb5 3.155(3) . ?
Mo19 Sb3 3.159(4) . ?
Mo20 O51 1.689(12) . ?
Mo20 O77 1.876(15) . ?
Mo20 O69 1.901(12) . ?
Mo20 O68 1.964(14) . ?
Mo20 O65 2.036(13) . ?
Mo20 O62 2.359(12) . ?
Mo20 Sb3 3.208(3) . ?
Mo21 O49 1.725(12) . ?
Mo21 O76 1.850(13) . ?
Mo21 O71 1.931(15) . ?
Mo21 O60 2.020(14) . ?
Mo21 O53 2.094(14) . ?
Mo21 O70 2.432(12) . ?
Mo21 Sb3 3.246(3) . ?
Mo22 O47 1.729(12) . ?
Mo22 O67 1.887(14) . ?
Mo22 O72 1.893(14) . ?
Mo22 O42 2.032(14) . ?
Mo22 O74 2.037(15) . ?
Mo22 O63 2.424(12) . ?
Mo22 Sb4 3.231(3) . ?
Mo23 O48 1.703(14) . ?
Mo23 O66 1.896(11) . ?
Mo23 O76 1.932(13) . ?
Mo23 O44 2.066(15) 4_344 ?
Mo23 O61 2.066(14) 4_344 ?
Mo23 O58 2.383(14) . ?
Mo23 Sb6 3.220(4) 4_344 ?
Mo24 O55 1.694(13) . ?
Mo24 O67 1.891(14) . ?
Mo24 O69 1.905(11) . ?
Mo24 O59 1.962(16) 4_344 ?
Mo24 O73 2.061(13) 4_344 ?
Mo24 O62 2.353(13) . ?
Mo24 Sb6 3.212(4) 4_344 ?
Sb1 O19 1.993(13) . ?
Sb1 O19 1.993(13) 2_455 ?
Sb1 O17 2.140(13) . ?
Sb1 O17 2.140(13) 2_455 ?
Sb2 O36 1.951(12) . ?
Sb2 O30 2.065(13) . ?
Sb2 O35 2.129(14) . ?
Sb2 O29 2.145(14) . ?
Sb3 Sb3 1.423(5) 2_454 ?
Sb3 O53 2.043(14) . ?
Sb3 O68 2.159(13) . ?
Sb3 O65 2.268(13) . ?
Sb3 O60 2.325(14) . ?
Sb4 Sb4 1.491(5) 2_354 ?
Sb4 O74 2.025(14) . ?
Sb4 O64 2.122(12) . ?
Sb4 O80 2.228(13) . ?
Sb4 O42 2.327(15) . ?
Sb5 Sb6 1.439(4) . ?
Sb5 O78 2.057(14) . ?
Sb5 O79 2.101(17) . ?
Sb5 O43 2.289(14) . ?
Sb5 O54 2.307(14) . ?
Sb6 O44 2.083(16) . ?
Sb6 O59 2.100(16) . ?
Sb6 O73 2.237(12) . ?
Sb6 O61 2.268(14) . ?
Sb6 Mo18 3.138(3) 4_354 ?
Sb6 Mo17 3.140(3) 4_354 ?
Sb6 Mo24 3.212(4) 4_354 ?
Sb6 Mo23 3.220(4) 4_354 ?
Sb7 O9 2.004(12) . ?
Sb7 O9 2.004(12) 2_455 ?
Sb7 O15 2.178(12) . ?
Sb7 O15 2.178(12) 2_455 ?
Si1 O2 1.608(14) . ?
Si1 O2 1.608(14) 2_455 ?
Si1 O18 1.621(12) 2_455 ?
Si1 O18 1.621(12) . ?
Si2 O32 1.597(13) 2_355 ?
Si2 O32 1.597(13) . ?
Si2 O27 1.625(13) 2_355 ?
Si2 O27 1.625(13) . ?
Si3 O62 1.647(13) . ?
Si3 O58 1.664(15) . ?
Si3 O70 1.670(13) . ?
Si3 O63 1.677(13) . ?
O9 Mo4 2.102(12) 2_455 ?
O10 Mo4 1.861(12) 2_455 ?
O13 Mo6 1.820(12) 2_455 ?
O19 Mo6 2.116(11) 2_455 ?
O26 Mo12 1.836(12) 2_355 ?
O29 Mo11 2.051(14) 2_355 ?
O29 Mo12 2.125(14) 2_355 ?
O30 Mo12 2.111(13) 2_355 ?
O36 Mo11 2.077(12) 2_355 ?
O40 Mo10 1.941(11) 2_355 ?
O44 Mo17 1.889(14) 4_354 ?
O44 Mo23 2.066(15) 4_354 ?
O59 Mo24 1.962(16) 4_354 ?
O59 Mo18 1.975(16) 4_354 ?
O61 Mo18 1.937(14) 4_354 ?
O61 Mo23 2.066(14) 4_354 ?
O73 Mo17 1.949(13) 4_354 ?
O73 Mo24 2.061(13) 4_354 ?
N1 C1 1.470(16) . ?
N2 C2 1.508(15) . ?
N3 C3 1.469(16) . ?
N4 C4 1.480(16) . ?
N5 C5 1.432(19) . ?
N6 C6 1.41(2) . ?
C1 C2 1.440(15) . ?
C3 C4 1.432(16) . ?
C5 C6 1.429(19) . ?
